Download presentation

Presentation is loading. Please wait.

Published byJasmine Sharp Modified over 2 years ago

1
First-principles calculations of diffusion coefficients in magnetic systems: Ni, Cr, and Ni-X alloys Chelsey Zacherl, Shun-Li Shang, and Zi-Kui Liu NIST Diffusion Workshop May 4 th, 2012 Acknowledgement: Office of Naval Research (ONR) under contract No. N0014-07-1- 0638 and the Center for Computational Materials Design (CCMD), a joint National Science Foundation (NSF) Industry/University Cooperative Research Center at Penn State (IIP-1034965) and Georgia Tech (IIP-1034968).

2
Outline Current challenges in diffusion by first- principles Ni self-diffusion (fcc) – Ferromagnetic calculations Cr self-diffusion (bcc) – Anti-ferromagnetic calculations Impurity diffusion in Ni-X binary alloys – 26 Ni-X systems Non-dilute diffusion in Ni-Al fcc system Summary and future work 2

3
Current challenges in calculating diffusion by first-principles Vibrational properties at the saddle point – SOLUTION: Eyring’s reaction rate theory and Nudged-Elastic Band (NEB) method Experimental self-diffusion data for Ni, Cr exists above magnetic transition temperature – Calculations performed with magnetic ordering Effect of magnetic ordering and disordering such as in Ni and Ni alloys – Empirical magnetic terms – Partition function/quantum Monte Carlo approach 3

4
Self-diffusion in cubic systems Vacancy-mediated In Arrhenius form: f – jump correlation factor a 2 – lattice parameter C – vacancy concentration w – atom jump frequency D 0 – diffusion prefactor (intercept) Q – activation energy (slope) k B – Boltzmann's constant 4 Mehrer, Diffusion in Solids, 2007

5
Initial vacancy configuration Vacancy mediated self-diffusion in fcc Ni: calculating the least energy diffusion path within Eyring’s reaction rate theory Saddle configuration 5 Mantina, PSU Dissertation, 2008 Ni 1 3 2 Eyring, J. Chem. Phys. 1935 Vacancy formation and migration:

6
Fcc Ni self-diffusion coefficients calculation input details Vienna ab-inito Simulation Package (VASP) Automated Theoretical Alloy Toolkit (ATAT) or Debye-Grüneisen model for finite temperature vibrational contribution 32-atom Ni supercell (2 x 2 x 2) Ferromagnetic spin on all atoms PAW-LDA Full relaxation of perfect and equilibrium vacancy configurations Nudged-Elastic Band (NEB) method for saddle point configurations No surface corrections used 6

7
Underestimation of diffusion parameters compared to experiments is a consistent trend in the present work Zacherl, Acta Mat., Under review, 2012 7

8
QHA Debye model approach yields better agreement with experiments than QHA phonon method 8 **Filled data points: Single-crystal **Open data points: Poly-crystal Zacherl, Acta Mat., Under review, 2012

9
Tabulated data yields same results regarding QHA Debye vs QHA Phonon MethodReferencesD 0 (m 2 /sec)Q (eV)T (K) DFT LDA QHA Debye (FM) The present work 1.99 x 10 -5 – 2.14 x 10 -4 2.85 – 3.03700 - 1700 DFT LDA Debye QHA (NM) The present work 5.27 x 10 -6 – 3.92x 10 -5 2.64 – 2.69700 - 1700 DFT LDA QHA Phonon (FM) The present work 3.90 x 10 -6 – 8.98 x 10 -6 2.80 - 2.79700 - 1700 DFT LDA HA Phonon (NM) Mantina 7.00 x 10 -6 – 7.09 x 10 -6 2.65 – 2.66700 - 1700 Expt. (SC)Bakker1.77 x 10 -4 2.9951253 - 1670 Expt. (SC)Vladimirov0.85 x 10 -4 2.871326 - 1673 Expt. (SC)Maier1.33 x 10 -4 2.91815 - 1195 9 Zacherl, Acta Mat., Under review, 2012

10
Non-magnetic calculations show worse results than ferromagnetic calculations for both methods 10 Debye Phonon Campbell, Acta Materialia, 2011

11
Thermodynamic properties of QHA FM LDA Debye compare well with experimental data 11 Ferromagnetic Nonmagnetic Zacherl, Acta Mat., Under review, 2012

12
Magnetization charge density shows mag- netic influence on thermodynamic properties 12 High Low PerfectInitial vacancy (corners)Saddle configuration Looking down b axis (spin up – spin down) Zacherl, Acta Mat., Under review, 2012

13
Diffusion of bcc AFM Cr shows good agreement with single-crystal data 13 **Filled data points: Single-crystal **Open data points: Poly-crystal

14
Arrhenius parameters of Cr self- diffusion MethodReferences D 0 * 10 4 (m 2 /sec) Q (eV)T (K) DFT PBE HA Phonon The present work 41.204.051000 145.84.112000 Expt: Single crystal Mundy, 19769704.511369-2093 Expt: Single crystal Mundy, 1981404.581073-1446 14

15
Conclusions from self-diffusion work in magnetic systems Magnetic effects are far reaching throughout supercell and affect thermodynamic properties Overestimation of energy of vacancy regardless of X-C functional used – Surface effect magnified by magnetic properties of fcc Ni Empiricism of the Debye model makes up for magnetic effects phonon is not representing – “double correction” 15

16
Dilute impurity diffusion in fcc ferromagnetic Ni-X alloys * Experimental dilute impurity diffusion data 16

17
Approach: impurity diffusion in Ni-X determined from jump frequency of the impurity atom, w 2 LeClaire and Lidiard’s five frequency model 17 LeClaire, Phil. Mag., 1956 Mehrer, Diffusion in Solids, 2007 Impurity correlation factor

18
Validation of methodology by comparing Q, activation barrier for diffusion to previous 0 K study Janotti, Physical Review Letters, 2004 18

19
Test system: LDA QHA Debye model for vibrational contribution, no electronic used **Filled data points: Single-crystal **Open data points: Poly-crystal Ni-Cu 19

20
Arrhenius parameters including temperature dependence at all temperatures D 0 (10 -4 m 2 /sec)Q (eV)T (K) This work – LDA Debye 0.0042.58700 0.0882.581700 Expt., Monma, 1964 0.572.6761327 – 1632 Expt., Anand, 19650.662.6451123 – 1323 Expt., Helfmeier, 1970 0.272.6461048 – 1323 Expt, Taguchi, 1984 0.612.6411080 – 1613 20

21
Results from selected impurity diffusion coefficient calculations Ni-Al Ni-Ti **Filled data points: **Open data points: Single-crystal Poly-crystal 21

22
Results from selected impurity diffusion coefficient calculations 22 **Filled data points: **Open data points: Single-crystal Poly-crystal Ni-Fe Ni-Cr

23
Results from selected impurity diffusion coefficient calculations **Filled data points: **Open data points: Single-crystal Poly-crystal 23

24
Comments on the Ni-X impurity diffusion results Underestimation of one order of magnitude compared to experimental data is consistent for all systems shown – Affecting activation barrier for diffusion, Q and diffusion prefactor, D 0 – Partially attributed to lack of complete relaxation of the three transition states in VASP Lingering question: – How to analyze data from 26 systems – Charge density 24

25
Full relaxation in VASP 5 using ss-CINEB TST tools from UT Austin shows slight correction at lower temperatures **Filled data points: Single-crystal **Open data points: Poly-crystal 25 Henkelman, Chem. Phys. 2000

26
How can we provide understanding of the effects of each X on the impurity diffusion coefficient? 26

27
Relative charge density analysis of Ni-Re compared to that of pure Ni 27 Pure Ni: Saddle configuration High Low Pure Ni: Saddle configuration a axisc axisb axis (spin up – spin down)

28
Relative charge density analysis of Ni-Y compared to that of pure Ni 28 Pure Ni: Saddle configuration High Low Pure Ni: Saddle configuration a axisc axisb axis (spin up – spin down)

29
Additional challenge: non-dilute impurity diffusion of Al in fcc FM Ni Bocquet’s 14 frequency model to predict all possible vacancy interactions with lone or paired solute atoms LeClaire’s 5 frequency model for lone solute atom – vacancy interactions Bocquet, Report: CEA-R-4292, 1972 Le Claire, J. Nuclear Mater. 69-70(1978) 70 Open circle: solvent Filled circle: solute Square: vacancy 29

30
14 Frequency model Calculations completed for Ni-Al system – 30 Ni atoms and 2 Al atoms – Solvent enhancement factor, b 1 – Solute enhancement factor, B 1 – Isotope effect measurement, E Current progress: – Empirical relation for impurity diffusion coefficient dependent on concentration: LeClaire, Journal of Nuclear Materials, 1978 30

31
Impurity diffusion coefficient for 26 FM Ni-X alloy systems – Deformation charge density – Trends in data Future: 14-frequency model – Fit to Redlich-Keister polynomial All calculations: limitations of magnetic model in comparison to experimental data – Did not include transition effects; shown to be less for Ni than other elements like Co or Fe – Debye vs. Phonon methods Conclusions and future work for this project 31 Shang, J. Appl. Phys., 2010Kormann, PRB, 2011 NiFe

32
Thank you! 32

33
Phonon calculations Based on the partition function of lattice vibrations, we have the phonon frequency as a function, g( ) 33 Shang, Acta. Mat., 2005 Wang, Acta. Mat., 2004 Phonon frequencyPhonon density of states

34
Debye-Grüneisen Model Speed of sound is constant in a material Linear density of states 34 Debye function: Debye - Grüneisen model for finding (D) and solving above equation: Shang, Comp. Mat. Sci., 2010 Moruzzi, Phys. Rev. B., 1988 Zero-point energy from lattice vibrations Grüneisen constant

35
Eyring’s Reaction Rate Theory Partition function Atom jump frequency * remove the imaginary frequency of the saddle configuration Eyring, J. Chem. Phys., Vol.3, 1935, 107 35

36
Fcc Ni self-diffusion coefficients calculation input details Vienna ab-inito Simulation Package (VASP) Automated Theoretical Alloy Toolkit (ATAT) or Debye-Grüneisen model for vibrational contribution 32-atom Ni supercell (2 x 2 x 2) Ferromagnetic spin on all atoms PAW-LDA or PAW-PBEsol Full relaxation of perfect, and equilibrium vacancy configurations Nudged-Elastic Band (NEB) method for saddle point configurations 36

37
Diffusion coefficient equations Mantina, Defect and Diffusion Forum, 2009

38
Ni NM diffusion coefficient by harmonic phonon calculations Mantina, PhD. Thesis, Penn State University, 2008

39
bcc Cr self-diffusion coefficients calculation input details Vienna ab-inito Simulation Package (VASP) Debye-Grüneisen model for vibrational contribution 54-atom Cr supercell (2-atom bcc base) – Spin of +/- 1.06 B /atom Anti-ferromagnetic spin PAW-GGA-PBE Full relaxation of perfect and equilibrium vacancy configurations Nudged-Elastic Band (NEB) method for saddle point configurations – Full relaxation 39

40
Impurity diffusion coefficient calculation input details Vienna ab-inito Simulation Package (VASP) 32 atom, supercell, N-2 Ni atoms, 1 impurity, 1 vacancy 8 total configurations Ferromagnetic spin on all atoms PAW-LDA Full relaxation of perfect, and equilibrium vacancy configurations NEB or Climbing Image Nudged-Elastic Band (CINEB) method for saddle point configurations – Relax only ionic positions Debye model for vibrational contribution 40

41
Impurity diffusion coefficient determined from the jump frequency of the impurity atom, w 2 Equation for impurity diffusion is related to tracer diffusion: With vacancy concentration and jump frequency: And the binding energy with impurity, X, and vacancy, V: LeClaire, J. Nuclear Matls, 1978 Wolverton, Acta Mat., 2007 41

42
Calculation of the impurity correlation factor, f 2, involves calculating all five jump frequencies f 2 is related to the probability of the impurity atom making the reverse jump back to its previous position Where F is the “escape probability” that after a dissociation jump, the vacancy will not return to a first nearest neighbor site of the impurity Mehrer, Diffusion in Solids, 2007 Manning, Physical Review, 1964 x = w 4 /w 0 42

43
Impurity diffusion coefficient for Ni-Si and Ni-Ti systems Ni-Si Ni-Ti **Filled data points: **Open data points: Single-crystal Poly-crystal 43

44
Impurity diffusion coefficient for Ni-Nb and Ni-Zr systems **Filled data points: **Open data points: Single-crystal Poly-crystal Ni-Nb Ni-Zr 44

45
Impurity diffusion coefficient for Ni-W and Ni-V systems **Filled data points: **Open data points: Single-crystal Poly-crystal Ni-W Ni-V 45

46
Other impurity elements

47
3d transition elements in Ni 47

48
4d transition elements in Ni 48

49
5d transition elements in Ni 49

50
LeClaire’s 5 freqnecies (1) w 0 : solvent–vacancy exchange frequency (far from a solute atom). (2) w 1 : solvent–vacancy exchange frequency for the rotational jump around one single solute atom (3) w 3 : solvent–vacancy exchange frequency for the solute–vacancy dissociative jump (4) w 4 : solvent–vacancy exchange frequency for the solute–vacancy associative jump (5) w 2 : single solute–vacancy exchange frequency

51
Bocquet’s 14 frequencies (6) w 33 : solvent–vacancy exchange frequency for the jump that takes the vacancy away from the solute pair (7) w 34 : solvent–vacancy exchange frequency for the jump that takes the vacancy away from one solute atom in the single atom configuration but at the same time brings the vacancy into the nearest neighbor position for the other solute atom (8) w 44 : solvent–vacancy exchange frequency for the jump that brings the vacancy to the nearest neighbor position for the solute pair (9) w 14 : solvent–vacancy exchange frequency for the jump that brings the vacancy from the nearest neighbor position to one of the solute atoms in the pair configuration to the nearest neighbor position of both solute atoms in the pair configuration.

52
Bocquet’s 14 frequencies, con’t (10) w 13 : solvent–vacancy exchange frequency for the jump that takes the vacancy from the nearest neighbor position to both solute atoms in the pair configuration to the nearest neighbor position to one of the solute atoms in the pair configuration. (11) w 11 : solvent–vacancy exchange frequency for the jump that keeps the vacancy at the nearest neighbor position to both solute atoms in the pair configuration. (12) w 23 : solute–vacancy exchange frequency for the jump that takes a solute atom away from the other solute (13) w 21 : solute–vacancy exchange frequency for a solute rotational jump around the other solute atom (14) w 24 : solute–vacancy exchange frequency for the jump that brings a solute atom to the nearest neighbor position of the other solute atom

Similar presentations

OK

Materials Process Design and Control Laboratory ON THE DEVELOPMENT OF WEIGHTED MANY- BODY EXPANSIONS USING AB-INITIO CALCULATIONS FOR PREDICTING STABLE.

Materials Process Design and Control Laboratory ON THE DEVELOPMENT OF WEIGHTED MANY- BODY EXPANSIONS USING AB-INITIO CALCULATIONS FOR PREDICTING STABLE.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on nuclear family and joint family in india Download ppt on coordinate geometry for class 9th 2015 Ppt on area and perimeter for class 4 Ppt on holographic technology in education Ppt on limitation act ontario Ppt on sustainable agriculture in india A ppt on computer networking Head mounted display ppt on tv Ppt on 2 stroke ic engines Ppt on 10 sikh gurus sikhism